Int. J. Electrochem. Sci., 7 (2012) 12064 - 12077 International Journal of ELECTROCHEMICAL SCIENCE www.electrochemsci.orgSynthesis, Characterisation and Evaluation of IrO2 BasedBinary Metal Oxide Electrocatalysts for Oxygen EvolutionReactionC. Felix, T. Maiyalagan*, S. Pasupathi*, B. Bladergroen, V. LinkovSouth African Institute for Advanced Materials Chemistry (SAIAMC), University of the WesternCape, Modderdam Road, Bellville 7535, Cape Town, South Africa* E-mail: firstname.lastname@example.org; email@example.comReceived: 13 June 2012 / Accepted: 29 September 2012 / Published: 1 December 2012IrO2, IrxRu1-xO2, IrxSnx-1O2 and IrxTax-1O2 (1 ≥ x ≥ 0.7) were synthesized, characterised and evaluatedas electrocatalysts for the oxygen evolution reaction in solid polymer electrolyte electrolysers. Theelectrocatalysts were synthesised by adapting the Adams fusion method. The physical properties of theelectrocatalysts were characterised by scanning electron microscopy, transmission electron microscopyand x-ray diffraction. Electrochemical activity of the electrocatalysts toward the oxygen evolutionreaction was evaluated by cyclic voltammetry and chronoamperometry. X-ray diffraction revealed nophase separation when RuO2 or SnO2 was introduced into the IrO2 lattice suggesting that solidsolutions were formed. Transmission electron microscope analysis revealed nanosize particles for allsynthesised metal oxides. Crystallinity increased with the addition of RuO2 and SnO2 while asuppression of crystal growth was observed with the addition of Ta2O5 to IrO2. Chronoamperometryrevealed that the addition of all the secondary metal oxides to IrO2 resulted in improved catalyticperformance. Ir0.7Ru0.3O2 was identified as the most promising electrocatalyst for the oxygen evolutionreaction.Keywords: Adams fusion method, Anodic electrocatalyst, Oxygen evolution reaction, Solid polymerelectrolyte, Water electrolysis.1. INTRODUCTION Solid polymer electrolyte (SPE) or commonly known as proton exchange membrane (PEM)electrolysers have in recent years received considerable interest as a production method for carbon freehydrogen [1 - 3]. SPE electrolysers are well suited for water electrolysis using intermittent powersources and have been identified by the European Commission as a key technology to transform
Int. J. Electrochem. Sci., Vol. 7, 2012 12065renewable electricity into hydrogen and oxygen . The main drawback at present is the high costassociated with the SPE electrolyser components such as the expensive precious metal electrocatalystsand proton conducting membranes [5, 6]. One way to reduce the cost of the SPE electrolyser is byimproving the specific performance and durability of the noble metal electrocatalysts. The oxygenevolution electrode (anode) is the greatest source of overpotential of the system at typical operatingcurrent density [2, 6] therefore the anodic electrocatalyst needs to be highly stable and active under theoperating conditions . IrO2 is commonly employed as the anodic electrocatalyst as it exhibits a highcorrosion resistance to the oxygen evolution reaction (OER) in a strong acidic environment [7, 8]. IrO2is scarce and very expensive , adding significantly to the cost of the SPE electrolyser system. Sincethere is still no non-metal electrocatalyst with satisfactory activity and durability, it becomes importantto improve both the activity and durability of the IrO2 electrocatalyst. The most common method ofenhancing the electrochemical properties of the IrO2 electrocatalyst is by insertion of other metaloxides into the IrO2 lattice. In this study, IrO2, IrxRu1-xO2, IrxSnx-1O2 and IrxTax-1O2 (1 ≥ x ≥ 0.7) weresynthesised and characterised as suitable anodic electrocatalysts for the SPE electrolyser. RuO2 isknown to be the most active towards the OER but suffers from instability, and should thus be stabilisedwith another metal oxide such as IrO2 or SnO2 [10, 11]. Corrosion of Ru proceeds via RuO4 and isdirectly coupled to oxygen evolution via this common intermediate. The stabilisation of Ru by Ir hasbeen explained on the basis of shifted oxidation potentials and surface segregation . IrO2 thusstabilises RuO2 by preventing its oxidation to the soluble RuO4 . Ir-Ru mixed oxides are known tohave superior catalytic and stability properties with respect to Ru-Ti mixed oxide electrodes . Ta isa well known addition to the dimensionally stable anode (DSA) electrodes and Ir-Ta oxides have beensuggested to be an efficient catalyst for the OER in acidic media due to the high activity and corrosionresistance . The IrO2-Ta2O5 system as DSAs is a promising catalyst in various electrochemicalindustries, such as cleaning of waste water and electrowinning (electro-extraction) of metals, whereoxygen evolution is the main anodic reaction. However Ta2O5 is mainly added to improve the servicelife of IrO2, which is the active and most expensive component . IrO2-Ta2O5 with the compositionof 70 % IrO2 and 30% Ta2O5 has been previously verified to be the best combination in binary metaloxide systems in present commercial applications . Sn was selected on the basis of its highchemical and mechanical stability as well as its lower cost than the expensive noble metals . TheAdams fusion method was adapted to synthesise the Ir based metal oxides and the electrocatalyticactivities were evaluated by cyclic voltammetry (CV) and chronoamperometry (CA). Physicalcharacterisation was performed by scanning electron microscope (SEM), transmission electronmicroscope (TEM) and x-ray diffraction (XRD).2. EXPERIMENTAL DETAILS2.1 Preparation of the catalyst The Adams fusion method, first described by R. Adams and R.L. Shriner , entails thefusion of the metal chloride precursor with NaNO3 in air at elevated temperatures. The method has
Int. J. Electrochem. Sci., Vol. 7, 2012 12066since been used to synthesise various noble metal oxides [15, 17-19]. H2IrCl6 (SA precious metals,South Africa), RuCl3, SnCl2.2H2O and TaCl5 (Alfa Aesar, Johnson Matthey) were used as catalystprecursors to synthesise the electrocatalysts. The catalyst precursor(s) were dissolved in 10 mlisopropanol (Alfa Aesar, Johnson Matthey) until a metal concentration of 3.5 x 10 -2 M was achievedand magnetically stirred for 90 minutes. For each type of binary metal oxide system the second metal(Sn, Ru or Ta) was added in a concentration of 5–30 mol % to Ir. Five grams of finely ground NaNO3(Holpro Fine Chemicals, South Africa) was added to the solution, which was then further stirred for 30minutes. The mixture was then dried in an oven for 30 minutes. The dried catalyst precursor/saltmixture was then reacted in a furnace for 120 minutes at 350 °C. No additional annealing stepfollowed to limit the sintering of the nanosize particles. The obtained metal oxide was cooled andwashed with ultrapure water to remove the unreacted NaNO3. The final step was to dry the metal oxidein an oven for 120 minutes at 100 °C.2.2 Preparation of the working electrode A predetermined size of Ti mesh (Bekinit K.K, Japan) was etched and cleaned by boiling inoxalic acid (NT Laboratory Supplies) for 12 minutes. Catalyst inks were prepared by mixing togetherthe synthesised metal oxides, 5 wt% Nafion solution (Aldrich) and ultrapure water in a ratio of 1:6:2.A measured volume of isopropanol was added to serve as dispersion medium. The mixture wasultrasonically dispersed for 30 minutes. An airbrush with N2 propulsion was used to spray the catalystink (1 mg cm-2) onto the pre-treated Ti mesh. The catalyst ink was thoroughly dried between eachlayer sprayed to prevent agglomeration of the electrocatalytic particles. Spraying of the catalyst layerwas followed by spraying a Nafion layer (1 mg cm-2). The working electrode was cut out with a punchand had an area of 0.785 cm2.2.3 Physical characterisation Physical phases and structures of the electrocatalysts were characterised by X-ray diffraction(XRD) employing the Bruker AXS D8 Advance diffractometer using Cu K radiation (λ = 1.5406 Å)operating at 40 kV and 40 mA. Scanning electron micrographs were obtained with the Hitachi X-650SEM using GENESIS software, working at 25 keV. Transmission electron micrographs were obtainedusing a Tecnai G2 F20 X-Twin Mat200 kV Field Emission TEM, operating at 200 kV.2.4 Electrochemical characterisation Electrochemical analyses were performed in a standard three-electrode cell at 25 oC andatmospheric pressure. The Ti mesh working electrode (as described in earlier), a 3M Ag/AgClreference electrode, a Pt mesh counter electrode and a 0.5 M H2SO4 electrolyte solution was used.Autolab potentiostat PGSTAT20 (Eco-Chemie) was used for CV and CA analyses to evaluate theelectrocatalytic activity of the synthesised electrocatalysts towards the OER. The electrolyte solution
Int. J. Electrochem. Sci., Vol. 7, 2012 12067was purged with N2 for 30 minutes before performing electrochemical measurements. CV wasperformed by cycling the potential from -0.2 to +1.2 V at a potential sweep rate of 50 mV s-1. CA wasperformed by stepping the potentials from 1.2 to 1.6 V and measuring the current (mA) response as afunction of time. Each potential step was performed for 30 minutes. All potentials are reported versusthe 3M Ag/AgCl electrode.3. RESULTS AND DISCUSSION3.1 Physical characterisation
Int. J. Electrochem. Sci., Vol. 7, 2012 12068 Figure 1. XRD patterns of (a) IrO2 (b) Ir0.7Ru0.3O2 (c) Ir0.9Sn0.1O2 and (d) Ir0.8Ta0.2Ox. Fig. 1 shows the XRD patterns of IrO2 and the best performing electrocatalysts (established byCA analysis) of the three metal oxide combinations i.e. Ir0.7Ru0.3O2, Ir0.9Sn0.1O2 and Ir0.8Ta0.2Ox. TheXRD analysis of IrO2 (Fig. 1a) revealed a rutile oxide characterised by an amorphous phase which isknown to consist of smaller particles. Calculated from the 101 phase using the Scherrer formula, theaverage particle size was estimated to be 3.5 nm. No metallic Ir was observed. The XRD analysis ofIr0.7Ru0.3O2 (Fig. 1b) revealed a crystalline structure assigned to tetragonal rutile. Sharper peaks wereobserved in comparison to pure IrO2 which indicates an increase in the particle size. The single peaksobserved at the 110 and 101 phases (2θ = 28° and 35° respectively) suggests that Ir 0.7Ru0.3O2 is a solid
Int. J. Electrochem. Sci., Vol. 7, 2012 12069solution of IrO2 and RuO2. This observation is consistent with other reports [8, 9, and 13]. The additionof RuO2 to IrO2 resulted in an increase in the 110 phase (a stable surface of IrO2) which may lead to asynergistic effect. Although it is known that IrO2 and RuO2 can form stable solid solutions, thepresence of multiple rutile phases should not be ruled out. The Hume–Rothery theory states that it ispossible to form a continuous solid solution of IrO2 and RuO2, where Ru4+ and Ir4+ share the same siteon the cationic sub-lattice of a tetragonal (rutile-like) phase . The higher degree of crystallisationobserved for Ir0.7Ru0.3O2 in comparison to pure IrO2 may be attributed to the fact that RuO2 crystallisesat a lower temperature than IrO2 . Calculated from the 110 and 101 phases using the Scherrerformula, the average particle size for Ir0.7Ru0.3O2 was estimated at 11 nm. The presence of metallic Irand Ru was not observed. Figure 2. SEM images of (a) IrO2 (b) Ir0.7Ru0.3O2 (c) Ir0.9Sn0.1O2 and (d) Ir0.8Ta0.2Ox.
Int. J. Electrochem. Sci., Vol. 7, 2012 12070 XRD analysis of Ir0.9Sn0.1O2 (Fig. 1c) revealed a rutile-type oxide with single peaks observed atthe 110 and 101 phases (2θ = 28° and 35° respectively) which suggests that Ir0.9Sn0.1O2 is a solidsolution of IrO2 and SnO2. The addition of SnO2 to IrO2 resulted in an increase in the 110 phase (astable surface of IrO2) which may lead to a synergistic effect. Mayousse et al.  also observed theformation of a solid solution between IrO2 and SnO2. They suggested that IrO2 and SnO2 crystallised inthe same tetragonal structure due to the comparable atomic radii of Ir and Sn. However the presence oftwo phases should not be ruled out. Marshall et al.  used profiling of the XRD patterns andsuggested that the XRD patterns were a mixture of two highly dispersed rutile oxide phases. Thepresence of multiple phases and the lack of a single solid solution phase were suggested to arise fromthe poor interaction of the precursors during the initial stages of the reaction. It was assumed that SnO 2formed first since there is a significant difference in ∆Gf0 for IrO2 and SnO2 (-510 kJ mol-1  and -186.5 kJ mol-1 , respectively). Calculated from the 110 and 101 phases using the Scherrer formula,the average particle size for Ir0.9Sn0.1O2 was estimated at 6.5 nm. The presence of metallic Ir and Snwas not observed. XRD analysis of Ir0.8Ta0.2Ox (Fig. 1d) revealed a slight decrease in the 110 phase of IrO2 and aslight increase in the 002 (one of the non-close-packed planes of the Ir atom) phase which is consistentwith what is reported in the literature . This could be explained by the stabilisation effect that Tahas on the Ir component in the non-close-packed plane . XRD analysis further revealed mainly anamorphous phase which is consistent with the results of Di Blasi et al . Calculated from 101 phaseusing the Scherrer formula, the average particle size for Ir0.8Ta0.2Ox was estimated at 3 nm. Theaddition of Ta2O5 is known to suppress the crystallisation of IrO2 . Ta was found to be present inthe +5 oxidation state; consistent to what was reported previously . The presence of metallic Ir andTa was not observed. Fig. 2 shows the SEM images of IrO2 and the best performing electrocatalysts (established byCA analysis) of the three metal oxide combinations i.e. Ir0.7Ru0.3O2, Ir0.9Sn0.1O2 and Ir0.8Ta0.2Ox.Particle formation and sizes could not be defined from the SEM images. The SEM image of IrO2 (Fig.2a) shows micrometer size flake shaped aggregates whereas Ir0.7Ru0.3O2 (Fig. 2b), Ir0.9Sn0.1O2 (Fig. 2c)and Ir0.8Ta0.2Ox (Fig. 2d) exhibited sheet like porous morphology. From the SEM images, it appearsthat the addition of the secondary metal oxides to IrO2 resulted in larger aggregate sizes. Fig. 3 shows the TEM images of IrO2 and the best performing electrocatalysts (established byCA analysis) of the three metal oxide combinations i.e. Ir0.7Ru0.3O2, Ir0.9Sn0.1O2 and Ir0.8Ta0.2Ox. TEManalysis of IrO2 (Fig. 3a) revealed an amorphous phase consisting of nanoparticles with an averagesize of about 4.5 nm. TEM analysis of Ir0.7Ru0.3O2 (Fig. 3b) revealed an amorphous phase consisting ofsmaller particles and a crystalline phase consisting of larger pin shaped particles of up to 80 nm inlength. The larger pin shaped particles formed due to the crystallisation of RuO2 as was revealed byXRD. TEM analysis of Ir0.9Sn0.1O2 (Fig. 3c) revealed an amorphous phase consisting of smallerparticles and a crystalline phase consisting of larger needle shaped particles of up to 50 nm in length.The larger needle shaped particles formed due to the crystallisation of SnO2 as was revealed by XRD.From literature [22, 27], a slight increase in particle size was observed as the SnO2 content wasincreased. The slight increase in particle size can be expected since the slightly larger Sn 4+ ions (0.083nm) are substituting the smaller Ir4+ ions (0.077 nm) in the IrO2 lattice . TEM analysis of
Int. J. Electrochem. Sci., Vol. 7, 2012 12071Ir0.8Ta0.2Ox (Fig. 3d) revealed uniformly distributed nanosize particles with an average size of 3.5 nm.The most important enhancing effect that the addition of Ta2O5 to IrO2 has is mainly related to thereduction of the particle size . Figure 3. TEM images of (a) IrO2 (b) Ir0.7Ru0.3O2 (c) Ir0.9Sn0.1O2 and (d) Ir0.8Ta0.2Ox.3.2 Electrochemical characterisation Fig. 4 shows the CV analysis for IrO2 and the best performing electrocatalysts (as establishedby CA analysis) of the three metal oxide combinations i.e. Ir0.7Ru0.3O2, Ir0.9Sn0.1O2 and Ir0.8Ta0.2Ox.The potential was cycled from -0.2 to +1.2 V (vs. 3M Ag/AgCl electrode) at a potential sweep rate of50 mV s-1 in 0.5M H3SO4 solution. The voltammetric curve for IrO2 (Fig. 4a) shows two peaks atabout 0.4 and 1 V which are located in the redox transition region . The peaks at 0.4 and 1V have
Int. J. Electrochem. Sci., Vol. 7, 2012 12072been assigned to redox couples Ir (III)/Ir (IV) and Ir (IV)/Ir (VI), respectively. There is a lack ofsymmetry along the potential axis especially in the region of the Ir (IV)/Ir (VI) redox couple which isprobably due to sluggish electrode kinetics.Figure 4. Cyclic voltammograms of (a) IrO2 (b) Ir0.7Ru0.3O2 (c) Ir0.9Sn0.1O2 and (d) Ir0.8Ta0.2Ox at 50 mVs-1. Furthermore the peaks are broad and not well depicted suggesting the existence of a variety ofactive surface sites with different formal potentials which is consistent with an amorphous state of IrO2. The voltammetric curve for Ir0.7Ru0.3O2 (Fig. 4b) shows a positive potential shift for the redoxtransition region in comparison to pure IrO2. The peak at about 0.6 and 0.95V was assigned to theredox transition couples of the Ru(III)/Ru(IV) and Ru(IV)/Ru(VI) respectively. The voltammogramdisplays reversible charge transfer transition in the O2 evolution region which suggests an
Int. J. Electrochem. Sci., Vol. 7, 2012 12073improvement in electrode kinetics in comparison to pure IrO2. At about -0.1V there is a noticeablepeak due to hydrogen adsorption which is commonly associated with the presence of a metallic speciessince hydrogen is not known to easily adsorb onto an oxide surface . However, no metallic Ir or Ruwas observed with XRD analysis. The voltammetric curve for Ir0.9Sn0.1O2 (Fig. 4c) exhibits a shapesimilar to that of pure IrO2 with a positive potential shift of the redox transition region which isobserved between 0.65 and 1.1V. The peak at about 0.65V can be assigned to the Ir(III)/Ir(IV) couplesince the electrode response is strongly dominated by the Ir component . The voltammogramshows good reversibility in the O2 evolution region suggesting improved electrode kinetics incomparison to pure IrO2. The voltammetric curve for Ir(0.8)Ta(0.2)Ox (Fig. 4d) displays two peaks at 0.7and 1.1V. The peak at about 0.7V is attributed to the Ir(III)/Ir(IV) couple which suggests that thesurface electrochemistry is governed by the active component of IrO2 . The voltammogram showsgood reversibility in the O2 evolution region suggesting improved electrode kinetics in comparison topure IrO2. CV was also used to investigate the electrochemical activities of the oxides which arerelated to the number of active sites accessible to the electrolyte solution . The anodic charge, qa,due to double layer charging and surface redox transitions, is proportional to the active site surfaceconcentration . Figure 5. Chronoamperometric measurements of IrO2 and IrxRu1-xO2 (1 ≥ x ≥ 0.7) at 1.6 V. The qa for the electrodes was obtained by integration of the voltammetric curves in the rangebetween H2 and O2 gas evolution. The qa values for IrO2, Ir0.7Ru0.3O2, Ir0.9Sn0.1O2 and Ir0.8Ta0.2Ox are144, 185, 180 and 274 mC cm-2, respectively. The mixed oxides show higher qa than for pure IrO2indicating that Ru, Sn and Ta have a positive effect on the active area of the mixed oxide electrodes. J-M Hu et al.  observed that the voltammetric charge significantly varies with the Ta compositionand that 20 mol % Ta addition shows a significantly higher charge value than that of pure IrO 2. The
Int. J. Electrochem. Sci., Vol. 7, 2012 12074higher qa for Ir0.8Ta0.2Ox may also be due to the smaller particle sizes as was revealed by TEM andXRD. De Pauli et al.  suggested that the sharp decrease in charge value as the electrode surfacecomposition reached 100 mol % IrO2 was due to diminution or a reduction of the surface area. Fig. 5 shows the CA analysis of the IrxRu1-xO2 (1 ≥ x ≥ 0.7) electrocatalysts performed at 1.6 Vfor 30 minutes. CA revealed the best electrocatalytic activity towards the OER for Ir 0.7Ru0.3O2.Electrocatalytic activity towards the OER increased as the RuO2 content was increased. Thisobservation is consistent with an improvement in the oxide activity due to the larger exchange currentdensity of RuO2 compared to that IrO2 . The catalytic activity of Ir0.7Ru0.3O2 was significantlyhigher than that of pure IrO2. The addition of RuO2 to IrO2 was reported to result in a significantreduction in the overpotential . The addition of RuO2 of up to 80 mol% was also reported to yield anelectrocatalyst with high electrochemical activity while displaying good stability under the OER .The combination of RuO2 and IrO2 could thus facilitate a reduction in the required electrocatalystloading as well as a direct material cost reduction considering that Ir is more expensive than Ru. Figure 6. Chronoamperometric measurements of IrO2 and IrxSnx-1O2 (1 ≥ x ≥ 0.7) at 1.6 V. Fig. 6 shows the CA analysis of the IrxSnx-1O2 (1 ≥ x ≥ 0.7) electrocatalysts performed at 1.6 Vfor 30 minutes. CA revealed the best electrocatalytic activity towards the OER for Ir 0.9Sn0.1O2. Asignificant increase in electrocatalytic activity was observed as a Sn content of 10 mol% was reachedwhich is consistent with a higher qa value obtained from CV for Ir0.9Sn0.1O2 as compared to pure IrO2.Further addition of Sn resulted in a rapid decrease in the oxide performance. However, CA analysisstill revealed an improved performance for all IrO2-SnO2 electrocatalysts in comparison to pure IrO2.
Int. J. Electrochem. Sci., Vol. 7, 2012 12075Xu et al.  reported similar behavior for their RuO2-SnO2 electrocatalysts where the catalytic activityinitially increased followed by a dramatic decrease as the Sn content was increased. Marshall et al. reported a 10 – 15% decrease in the total active area for SnO2 contents of 20 – 30 mol% but alsoobserved a better cell performance for Ir0.8Sn0.2O2 as compared to pure IrO2 at 25°C . Xu et al. observed that at low SnO2 contents the IrO2 particles were well dispersed but at higher SnO2 contentsthe active surface area of IrO2 decreased due to an increase in the average particle size. Figure 7. Chronoamperometric measurements of IrO2 and IrxTax-1O2 (1 ≥ x ≥ 0.7) at 1.6 V. Fig. 7 shows the CA analysis of the IrxTax-1O2 (1 ≥ x ≥ 0.7) electrocatalysts performed at 1.6 Vfor 30 minutes. The best catalytic activity towards the OER was observed for Ir0.8Ta0.2Ox. An increasein electrocatalytic activity was observed as the Ta content was increased up to 20 mol% followed by adecrease in electrocatalytic activity as the Ta content reached 30 mol %. The addition of Ta2O5 to IrO2was reported to increase the resistivity by 2 orders of magnitude by the time the composition reachedIr0.7Ta0.3Ox, due to the low electronic conductivity of Ta2O5 . The catalytic activity for Ir0.7Ta0.3Oxwas still slightly higher than that of pure IrO2. It was previously suggested that an improved activesurface area can be obtained when there is a proper ratio of Ir to Ta . A similar trend inperformance was reported by Hu et al.  however they observed a maximum current response at 30mol% Ta content. Furthermore, a higher cell resistance was observed for the Ir-Ta oxides incomparison to other Ir based metal oxides . The improved electrocatalytic activity observed by theaddition of Ta2O5 to IrO2 was probably as a result of the smaller particle sizes (revealed by XRD andTEM) and increased active surface sites (revealed by CV).
Int. J. Electrochem. Sci., Vol. 7, 2012 120764. CONCLUSIONS Electrocatalysts based on IrO2 were successfully synthesised and characterised. CA analyseshave shown that the addition of secondary metal oxides (RuO2, SnO2 and Ta2O5) to IrO2, improved thecatalytic activity of the oxide towards the OER. Ir0.7Ru0.3O2, while displaying a slightly lower catalyticactivity than Ir(0.9)Sn(0.1)O2, proved to be the most promising electrocatalyst for the OER since nodecrease in catalytic activity was observed as the RuO2 content was increase up to 30 mol%. Thissuggests that even better catalytic activity may be achieved with even higher contents of RuO 2. Theaddition of SnO2 and Ta2O2 was limited to 10 and 20 mol% respectively. CA proved to be a usefultechnique for the electrochemical characterisation of the electrocatalysts. TEM and XRD were usefulin relating the physical structure of the electrocatalysts to the electrochemical activity. Particle sizeswere found to be of nanometer scale for all the synthesised electrocatalysts thus rendering the Adamsfusion method a relatively simple and quick method for directly producing metal oxides suitable aselectrocatalysts for the SPE electrolyser. The combination of various metal oxides can be considered aviable approach to address the high cost and efficiency issues facing the present SPE electrolysertechnology.ACKNOWLEDGEMENTSThis work was supported by the South African Department of Science and Technology through theTechnology Implementation Agency (TIA) project number T70600 (SPE Electrolyser).References1. W. Xu, J. Tayal, S. Basu, K. Scott, Int. J. Hydrogen Energy, 36 (2011) 14796.2. A.T. Marshall, S. Sunde, M. Tsypkin, R. Tunold, Int. J. Hydrogen Energy, 32 (2007) 2320.3. T. Maiyalagan, S. Pasupathi, Mater. Sci. Forum, 657 (2010) 143.4. C. Xu, L. Ma, J. Li, W. Zhao, Z. Gan, Int. J. Hydrogen Energy, (2011) 1.5. J. Cheng, H. Zhang, H. Ma, H. Zhong, Y. Zou, Electrochim. Acta, 55 (2010) 1855.6. S. Song, H. Zhang, X. Ma, Z. Shao, R.T. Baker, B. Yi, Int. J. Hydrogen Energy, 33 (2008) 4955.7. S. Siracusano, V. Baglio, A. Stassi, R. Ornelas, V. Antonucci, A.S. Arico, Int. J. Hydrogen Energy, 36 (2011) 7822.8. J. Cheng, H. Zhang, G. Chen, Y. Zhang, Electrochim. Acta, 54 (2009) 6250.9. E. Mayousse, F. Maillard, F. Fouda-Onana, O. Sicardy, N. Guillet, Int. J. Hydrogen Energy, 36 (2011) 10474.10. A.Marshall, B. Børresen, G. Hagen, M. Tsypkin, R. Tunold, Energy, 32 (2007) 431.11. A.Marshall, B. Børresen, G. Hagen, S. Sunde, M. Tsypkin, and R. Tunold, Russian J. Electrochem., 42 (10) (2006) 1134.12. R. Kötz, S. Stucki, Electrochim. Acta, 31 (10) (1986) 1311.13. W. Xu, K. Scott, S. Basu, J. Power Sources, 196 (2011) 8918.14. C. Angelinetta, S. Trasatti, Mater. Chem. Phys., 22 (1989) 231.15. E. Rasten, Electrocatalysis in water electrolysis with solid polymer electrolyte, PhD. Thesis, Norwegian University of Science and technology (2001).16. J.M. Hu, H.M. Meng, J.Q. Zhang, C.N. Cao, Corrosion Sci., 44 (2002) 1655.17. Y. Zhang, C. Wang, Z. Mao, N. Wang, Mater. Lett., 61 (2007) 1205.18. R. Adams, R.L. Shriner, J. Am. Chem. Soc., 45 (1923) 2171.